Initial stem cell adhesion on porous silicon surface: molecular architecture of actin cytoskeleton and filopodial growth
© Collart-Dutilleul et al.; licensee Springer. 2014
Received: 30 April 2014
Accepted: 25 July 2014
Published: 10 October 2014
The way cells explore their surrounding extracellular matrix (ECM) during development and migration is mediated by lamellipodia at their leading edge, acting as an actual motor pulling the cell forward. Lamellipodia are the primary area within the cell of actin microfilaments (filopodia) formation. In this work, we report on the use of porous silicon (pSi) scaffolds to mimic the ECM of mesenchymal stem cells from the dental pulp (DPSC) and breast cancer (MCF-7) cells. Our atomic force microscopy (AFM), fluorescence microscopy, and scanning electron microscopy (SEM) results show that pSi promoted the appearance of lateral filopodia protruding from the DPSC cell body and not only in the lamellipodia area. The formation of elongated lateral actin filaments suggests that pores provided the necessary anchorage points for protrusion growth. Although MCF-7 cells displayed a lower presence of organized actin network on both pSi and nonporous silicon, pSi stimulated the formation of extended cell protrusions.
In the field of regenerative medicine, tissue engineering offers promises for the treatment of various human diseases. Biologic tissues consist of cells, extracellular matrix (ECM), and signaling systems, activating genes or transcriptional factors responsible for tissue growth and differentiation. Thus, tissue engineering aims at recreating tissues that are defective or lost and is based on biological substitutes to repair physiological tissue functions by combining cells, bioactive factors, and biomaterial scaffolds. Cell-based therapies are driven by the observation that tissue or organ transplantation brings significant benefits to treated patients. Cell therapies are not only processing cells or tissues but also engineering and manufacturing cell-based products. Cellular engineering procedures motivate the development of scaffolds incorporating cell-level parameters such as endogenously produced factors and favorable physicochemical microenvironment. An essential challenge in tissue engineering is the understanding of cell-substrate interactions, which are involved in the difference observed in cell behavior when comparing in vitro and in vivo culturing[3, 4]. Indeed, stem cell-based therapies often require a scaffold to carry stem cells to the injured site. In human body, cells are in contact with each other and with ECM, all of them exhibiting nanostructures such as nanopores, nanofibers, or arrangements of adhesion proteins. Cell behavior is determined by intrinsic and extrinsic cell signals (from the surrounding cells and ECM). The extrinsic signals are of both chemical (bioactive molecules) and mechanical (forces caused by the cell-cell or cell-ECM interactions, at the micrometer and nanometer scale) nature. The way cells explore their surrounding ECM during development and migration is mediated by protrusion of actin-rich structures at the cell front. These protrusive structures are commonly called lamellipodium, which are built of a dense network of actin filaments. Lamellipodium protrusions are frequently accompanied by the formation of bundles of parallel actin filaments, usually termed filopodia. Lamellipodia frequently embed actin filament microspikes. These microspikes can develop into filopodia by protruding beyond the lamellipodium edge, but also as peripheral actin filament retraction fibers, associated with the sides of migrating cells. Filopodia are dynamic structures that rapidly extend and retract, found at the edge of various motile cells, as well as the growth cone tips of migrating axons. Cells use filopodia as sensor of the local environment to explore surfaces of other cells and surrounding ECM, in order to identify appropriate adhesion sites[7, 8]. A central concern of tissue engineering is to understand how to control the microenvironment surrounding the cells to restore similar conditions for cells as in their innate environment. For this, micropatterning has been used to create substrates with controlled architecture and optimized surface chemical properties. The topography of the substrate surface appeared to exert an effect on cells independently to surface chemistry. Thus, a biomaterial scaffold for tissue engineering should ideally mimic the chemical and mechanical properties of in vivo environment, in order to support cell attachment, proliferation, and differentiation. In this field, porous silicon (pSi) appears to be a promising biomaterial as it is both nontoxic and bioresorbable under physiological conditions and dissolves progressively into nontoxic silicic acid[5, 9, 10]. PSi is a semiconductor material obtained by electrochemical etching of flat silicon. Nanostructured pSi has been studied and used as a biomaterial with many advantages over existing alternatives as it is inorganic and can be readily sterilized. Pore dimensions can be controlled and tuned, from micropores (<2 nm) through mesopores (2 to 50 nm) to macropores (>50 nm up to several microns). It is well tolerated and noninflammatory within the body, and it has the ability to degrade completely in aqueous solutions into nontoxic silicic acid, the major form of silicon in the human body[11, 12]. Depending on the chemical doping of the silicon material base, conditions of fabrication and the surface functionalization applied, the degradation kinetics can vary from hours to months[10, 12]. And pSi has been shown to support the attachment and growth of a variety of mammalian cells[13–15]. Moreover, in physiological concentrations, it has been demonstrated that silicic acid stimulated collagen type I synthesis and osteoblast differentiation, highlighting the positive effect of Si on bone tissue healing. PSi structure has also been shown to favor calcium phosphate nucleation.
In vitro, interactions with the culture surface allow cells to respond to various mechanical forces, and surface porosity influences initial cell attachment and spreading, where cells attach to and pull on the matrix. Cell spreading can be described as a balance between cellular forces of protrusion, contraction, and adhesion. The micro- and nanoarchitecture plays an important role by promoting or not cell attachment and spreading.
Stem cell biology is an important field for the understanding of tissue regeneration and further regenerative medicine. Mesenchymal stem cells (MSCs) have been isolated first from bone marrow and then from various tissues, such as adipose tissue, umbilical cord blood, dental pulp, and many others. MSCs are adherent fibroblast-like cells able to proliferate in vitro and capable of giving rise to at least three cell lineages: osteogenic, chondrogenic, and adipogenic. The first type of dental stem cell was isolated from the human pulp tissue and named dental pulp stem cells (DPSCs). They have the ability to differentiate into various cell lineages, such as osteogenic, adipogenic, chondrogenic, neurogenic, myogenic, dentogenic, and cementogenic. Moreover, they are easily accessible after tooth extraction, especially wisdom teeth extraction for orthodontic reasons.
We aimed to study the influence of pSi porosity on cell adhesion, especially through lamellipodia and filopodia formation. The effect of pore size and porosity on cell growth is of particular relevance, as it will direct the fabrication of a porous biomaterial. Although microscale topography modulates cellular behavior in vitro, it is important to consider that cells in vivo make contact with nanoscale as well as microscale topographical features. Even if cells are typically tens of microns in diameter, the dimensions of subcellular structures tend to the nanometer scale[10, 23]. Therefore, we considered the impact of pSi porosity on cell adhesion and spreading. We investigated the behavior of primary culture of human DPSC on pSi scaffolds with pore diameters ranging from 30 to 40 nm. We focused on the formation of actin network and protrusions according to the presence of pores, using atomic force microscopy (AFM), fluorescence microscopy, and scanning electron microscopy (SEM). Nonporous silicon substrate (flat Si) and breast cancer (MCF-7) cell lines were used as controls. MCF-7 cell lines are a standard model of metastatic cancer cells, adherent, proliferative, and capable of living several months in vitro. Unlike MSCs, they are not able to differentiate and have limited spreading capacities[24, 25].
Porous silicon scaffolds
Porous silicon scaffolds were created from P++ type boron-doped crystalline silicon wafers with 0.0008 to 0.0012 Ω cm resistivity, obtained from Siltronix (Siltronix, Archamps, France). Wafers were etched in a custom-made Teflon cell at a constant current density of 300 mA/cm2 for 2 min 15 s, in a hydrofluoric acid (HF) solution in ethanol (3:1 HF/ethanol solution, volume ratio). Etched wafers were oxidized at 800°C for 1 h and cut into 0.5-cm2 pieces. Nonetched silicon wafers (flat Si) were also oxidized at 800°C for 1 h and used as control. To characterize pSi pore diameter, the topography of the surface was analyzed by environmental scanning electron microscopy (SEM) (Analytic FEI Quanta FEG 200, FEI, Hillsboro, OR, USA) with an acceleration voltage of 20.00 kV in a pressure of 0.5 Torr. SEM images were treated and analyzed using ImageJ® software to measure the mean pore diameter. For cell culture experiments, pSi and flat Si scaffolds were sterilized in 70% ethanol for 10 min, and cells were seeded onto the surface of sterilized pSi or flat Si at a density of 105 cell/mL.
Human dental pulp stem cells
Human impacted third molar extracted for orthodontic reasons were recovered from healthy patients (15 to 18 years of age), after written informed consent, following a protocol approved by the local ethical committee (Comité de Protection des Personnes, Montpellier hospital, France). Dental pulp cells were recovered after pulp enzymatic digestion in a solution of 3 mg/mL collagenase type I and 4 mg/mL dispase (BD Biosciences, Bedford, MA, USA). Cells were incubated for 1 week in 75-mL flasks, at 37°C with 5% CO2, in αMEM supplemented with 10% fetal bovine serum (Invitrogen, Carlsbad, CA, USA). Nonadherent cells were removed by a change of medium 24 h after cell seeding. After 1 week, subconfluent cells were collected and analyzed for minimal criteria to define human mesenchymal stem cells, such as adherence to plastic, expression of cell surface antigens, and ability to differentiate into osteoblasts, adipocytes, and chondroblasts in vitro.
We used MCF-7 breast cancer cell lines as a control in our experiments. MCF-7 cell lines were obtained from the American Type Culture Collection (ATCC, Manassas, VA, USA). Cells were cultured at 37°C in a humidified atmosphere with 5% CO2, in DMEM containing 4.5 g/L d-Glucose, supplemented with 10% fetal bovine serum (all from Invitrogen, Carlsbad, CA, USA).
Atomic force microscopy
An Asylum MFP-3D atomic force microscopy (AFM) system (Asylum Research, Santa Barbara, CA, USA), mounted on an Olympus inverted microscope (Olympus Corporation, Shinjuku-ku, Japan), was used for cell imaging. Triangular silicon nitride cantilevers (MLCT-AUHW, Veeco, Plainview, NY, USA) with a nominal spring constant of 10 pN/nm and half-opening angle of 40°, were used. The spring constant for each cantilever was determined by thermal noise method within the supplied software. Cells were examined after 24 h of in vitro incubation on pSi scaffolds or on flat Si. Cells were fixed in 2.5% glutaraldehyde for 1 h, then rinsed three times in phosphate buffer saline (PBS) (Invitrogen, Carlsbad, CA, USA). AFM topographic images were obtained using contact mode in liquid (PBS) at room temperature.
Cells were incubated for 24 h at 37°C with 5% CO2, in a humidified incubator, then fixed in 3.7% formaldehyde for 20 min at room temperature, and stained for actin cytoskeleton and nuclei. Cells were permeabilized with 0.5% Triton X-100 in PBS at 4°C for 15 min, incubated for 1 h with TRITC-labeled phalloidin (1:200) at 37°C in the dark, then with Hoechst 33342 (Life Technologies, Carlsbad, CA, USA) for 10 min at room temperature, and washed twice with deionized water. Samples were observed under fluorescence microscopy (Nikon TE2000, Nikon Instruments, Amsterdam, Netherlands) at an excitation wavelength of 360 nm for Hoechst staining (nucleus staining) and 630 nm for phalloidin (actin staining).
Scanning electron microscopy
Cells were cultured on pSi and flat Si scaffolds for 24 h under normal conditions, as described above. After incubation, cells were washed with PBS and fixed with 2.5% glutaraldehyde for 1 h at room temperature. Samples were dehydrated in graded ethanol solutions from 50 to 100% and in hexamethyldisilazane (HMDS, Ted Pella, Redding, CA, USA), then sputter-coated with platinum. Scanning electron microscopy (SEM) was performed on an Analytic FEI Quanta FEG 200 microscope (FEI, Hillsboro, OR, USA) with an acceleration voltage of 15 kV in a pressure of 1 × 10−5 Torr.
Results and discussion
PSi surface characterization
Cell morphology by SEM observation
Cell morphology is responsive to topographical features of the substrate surface, and the way cells adhere and spread on the surface influences their shape, growth, and differentiation. On both flat and porous surfaces, DPSCs spread widely with typical long axis size ranging from 60 to 80 μm and formed lamellipodia at the leading edge or even at both edges. SEM images of DPSCs on pSi and flat Si are presented in Figure 1.
Actin cytoskeleton observation
Filopodia characterization by AFM
The lateral filopodia were able to extend only on the porous surface leading to the hypothesis that pores provided anchorage points for protrusion growth and possible further cell spreading and crawling. The directional extension of lamellipodia on both surfaces modulated cell morphology, resulting in a fibroblast-like morphology. It has already been shown that cytoskeletal tension was related to the surface topography of substrates, with filopodia detecting surface topography, converting into lamellipodia and directing cell spreading and shape[35, 36]. DPSCs are multipotent stem cells able to give rise to multilineage differentiation[20, 21, 37, 38]. The investigation of the relationship between filopodia/lamellipodia formations, cytoskeletal tension, and surface nanopatterning aims to elucidate the impact of surface topography on cell spreading, migration, and further differentiation.
Role of filopodia on initial cell response to pSi surface
Filopodia have been shown to play an important role in cell migration: these thin actin protrusions can probe the extracellular environment and guide cell migration toward sites of interest. They can also be involved in other cellular processes such as wound healing, adhesion to the extracellular matrix, guidance toward chemoattractants, and neuronal growth-cone pathfinding. Filopodia are linked to the enhancement of directed cell migration, because they are essential components, with lamellipodia, for cell motility. This correlates with the role of filopodia in sensing the cell's surroundings and acting as sites for signal transduction. We showed in this study that porous surface had a strong impact on filopodia formation, as lateral actin protrusions were observed only on pSi and not on flat Si. Previous studies enlightened the influence of pSi nanoscale textured micropatterns on mesenchymal stem cell adhesion and migration, with cells migrating toward the porous areas. According to the pattern size, cellular filopodia can even bypass some unfavorable areas to reach some more suitable surfaces. The mechanisms underlying cell-topography interactions remain elusive but have a major impact on cell spreading and migration. These interactions concern not only porous structure but also various surface topographies. Similar results have recently been presented on microsphere array patterns promoting MSC adhesion and spreading through filopodia formation and conversion of filopodia into lamellipodia.
No organized actin structures were observed with MCF-7 on pSi and flat Si. These results are in accordance with previous published works, showing that actin structures in MCF-7 formed a disorganized network with few filaments at the basal plane of the cell. The presence of reduced organized actin filaments in MCF-7 was observed in this work as well and used as a negative control. However, some elongated thin protrusions growing from MCF-7 could be observed when the cells were incubated on pSi.
Cell-scaffold interactions play a significant role in tissue engineering to guide cell spreading and migration. Even if the mechanisms underlying these interactions remain elusive, we assume pSi porosity at the nanometer scale promotes environment exploration through filopodia formation and further cell migration. Filopodia can turn into lamellipodia to initiate the directional formation and extension of lamellipodia. Filopodia are not only acting as probes to detect microenvironment but also serve as skeleton to guide lamellipodia extension for directing cell motions, in response to surface topography. In our findings, it remains elusive whether filopodia appeared first and some of them guided the formation of lamellipodia or if lateral filopodia were probing microenvironment during cell migration toward the leading edge (where the lamellipodia is). Here, we show that filopodia contain a core of extending actin filament bundles. We assume that cell actively probes the external environment on pSi surface to gather spatial, topographical, and chemical information from the material surface. Such hair-like filopodial protrusions have been thought to locate specific ECM protein motifs and initiate integrin receptor clustering and focal adhesion protein recruitment, which is the first step of mature adhesion formation, before potential stem cell differentiation.
PSi is indeed a promising nanostructured biomaterial scaffold to be easily used in tissue engineering as it ideally mimics the ECM environment properties, in order to support cell attachment, development, and migration. Our work demonstrates that pSi plays an important role in promoting the formation of lateral actin microfilaments protruding from the DPSC cell body and from the lamellipodia area. Here, pSi porosity seems to provide the necessary anchorage points for filopodia growth. The observed lateral filopodia could act as supplementary probes to explore the surrounding environment. Moreover, control experiments showed that pSi permits the development of filopodia-like structures, even with MCF-7 cancerous cell lines. We believe these results might be of importance for tissue engineering applications. Further work is required and is currently on process to assess the impact of porosity on anchorage protein organization in vitro and the effect in vivo of such a biocomplex MSC-pSi.
The authors would like to acknowledge funding support from the Institut Francais pour la Recherche Odontologique (IFRO), France. The authors gratefully acknowledge Dr. Pierre Jacquemart for his kind help in elaborating the clinical procedure for wisdom teeth recovery.
- Bell E: Tissue engineering in perspective. In Principles of Tissue Engineering. Edited by: Lanza RP, Langer R, Vacanti J. San Diego, USA: Academic; 2000:3–7.Google Scholar
- Kirouac DC, Zandstra PW: The systematic production of cells for cell therapies. Cell Stem Cell 2008, 3: 369–381. 10.1016/j.stem.2008.09.001View ArticleGoogle Scholar
- Martinez E, Engel E, Planell JA, Samitier J: Effects of artificial micro- and nano-structured surfaces on cell behaviour. Ann Anat 2009, 191: 126–135. 10.1016/j.aanat.2008.05.006View ArticleGoogle Scholar
- Yim EKF, Leong KW: Significance of synthetic nanostructures in dictating cellular response. Nanomedicine 2005, 1: 10–21. 10.1016/j.nano.2004.11.008View ArticleGoogle Scholar
- Collart Dutilleul P-Y, Secret E, Panayotov I, Deville de Périère D, Martin-Palma RJ, Torres-Costa V, Martin M, Gergely C, Durand J-O, Cunin F, Cuisinier F: Adhesion and proliferation of human mesenchymal stem cells from dental pulp on porous silicon scaffolds. ACS Appl Mater Interfaces 2014, 6: 1719–1728. 10.1021/am4046316View ArticleGoogle Scholar
- Faix J, Rottner K: The making of filopodia. Curr Opin Cell Biol 2006, 18: 18–25. 10.1016/j.ceb.2005.11.002View ArticleGoogle Scholar
- Wood W, Martin P: Structures in focus—filopodia. Int J Biochem Cell Biol 2002, 34: 726–730. 10.1016/S1357-2725(01)00172-8View ArticleGoogle Scholar
- Kress H, Stelzer EHK, Holzer D, Buss F, Griffiths G, Rohrbach A: Filopodia act as phagocytic tentacles and pull with discrete steps and a load-dependent velocity. Proc Natl Acad Sci U S A 2007, 104: 11633–11638. 10.1073/pnas.0702449104View ArticleGoogle Scholar
- Park J-H, Gu L, von Maltzahn G, Ruoslahti E, Bhatia SN, Sailor MJ: Biodegradable luminescent porous silicon nanoparticles for in vivo applications. Nat Mater 2009, 8: 331–336. 10.1038/nmat2398View ArticleGoogle Scholar
- Collart Dutilleul P-Y, Deville de Périère D, Cuisinier FJ, Gergely C, Cunin F: Porous silicon scaffolds for stem cells growth And osteodifferentiation. In Porous Silicon for Biomedical Applications. Edited by: Santos H. Cambridge, UK: Woodhead Pub Limited; 2014:486–506.View ArticleGoogle Scholar
- Canham LT: Bioactive silicon structure fabrication through nanoetching techniques. Adv Mater 1995, 7: 1033–1037. 10.1002/adma.19950071215View ArticleGoogle Scholar
- Low SP, Voelcker NH, Canham LT, Williams KA: The biocompatibility of porous silicon in tissues of the eye. Biomaterials 2009, 30: 2873–2880. 10.1016/j.biomaterials.2009.02.008View ArticleGoogle Scholar
- Sapelkin AV, Bayliss SC, Unal B, Charalambou A: Interaction of B50 rat hippocampal cells with stain-etched porous silicon. Biomaterials 2006, 27: 842–846. 10.1016/j.biomaterials.2005.06.023View ArticleGoogle Scholar
- Low SP, Williams KA, Canham LT, Voelcker NH: Evaluation of mammalian cell adhesion on surface-modified porous silicon. Biomaterials 2006, 27: 4538–4546. 10.1016/j.biomaterials.2006.04.015View ArticleGoogle Scholar
- Alvarez SD, Derfus AM, Schwartz MP, Bhatia SN, Sailor MJ: The compatibility of hepatocytes with chemically modified porous silicon with reference to in vitro biosensors. Biomaterials 2009, 30: 26–34. 10.1016/j.biomaterials.2008.09.005View ArticleGoogle Scholar
- Hing KA, Revell PA, Smith N, Buckland T: Effect of silicon level on rate, quality and progression of bone healing within silicate-substituted porous hydroxyapatite scaffolds. Biomaterials 2006, 27: 5014–5026. 10.1016/j.biomaterials.2006.05.039View ArticleGoogle Scholar
- Canham LT, Reeves CL, Loni A, Houlton MR, Newey JP, Simons AJ, Cox TI: Calcium phosphate nucleation on porous silicon: factors influencing kinetics in acellular simulated body fluids. Thin Solid Films 1997, 297: 304–307. 10.1016/S0040-6090(96)09534-XView ArticleGoogle Scholar
- Miron-Mendoza M, Seemann J, Grinnell F: The differential regulation of cell motile activity through matrix stiffness and porosity in three dimensional collagen matrices. Biomaterials 2010, 31: 6425–6435. 10.1016/j.biomaterials.2010.04.064View ArticleGoogle Scholar
- Haridas V, Sadanandan S, Collart Dutilleul P-Y, Gronthos S, Voelcker NH: Lysine-appended polydiacetylenes scaffolds for human mesenchymal stem cells. Biomacromolecules 2013, 15: 582–590.View ArticleGoogle Scholar
- Gronthos S, Mankani M, Brahim J, Robey PG, Shi S: Postnatal human dental pulp stem cells (DPSCs) in vitro and in vivo. Proc Natl Acad Sci U S A 2000, 97: 13625–13630. 10.1073/pnas.240309797View ArticleGoogle Scholar
- Huang GT-J, Gronthos S, Shi S: Mesenchymal stem cells derived from dental tissues vs. those from other sources: their biology and role in regenerative medicine. J Dent Res 2009, 88: 792–806. 10.1177/0022034509340867View ArticleGoogle Scholar
- Atari M, Gil-Recio C, Fabregat M, García-Fernández D, Barajas M, Carrasco MA, Jung H-S, Alfaro FH, Casals N, Prosper F, Ferrés-Padró E, Giner L: Dental pulp of the third molar: a new source of pluripotent-like stem cells. J Cell Sci 2012, 125: 3343–3356. 10.1242/jcs.096537View ArticleGoogle Scholar
- Biggs MJP, Richards RG, Dalby MJ: Nanotopographical modification: a regulator of cellular function through focal adhesions. Nanomedicine 2010, 6: 619–633. 10.1016/j.nano.2010.01.009View ArticleGoogle Scholar
- Levenson AS, Jordan VC: MCF-7: the first hormone-responsive breast cancer cell line. Cancer Res 1997, 57: 3071–3078.Google Scholar
- Salehi H, Middendorp E, Panayotov I, Collart Dutilleul P-Y, Dutilleul P-YC, Vegh A-G, Ramakrishnan S, Gergely C, Cuisinier F: Confocal Raman data analysis enables identifying apoptosis of MCF-7 cells caused by anticancer drug paclitaxel. J Biomed Opt 2013, 18: 56010. 10.1117/1.JBO.18.5.056010View ArticleGoogle Scholar
- Dominici M, Le Blanc K, Mueller I, Slaper-Cortenbach I, Marini F, Krause D, Deans R, Keating A, Prockop D, Horwitz E: Minimal criteria for defining multipotent mesenchymal stromal cells. Int Soc Cell Ther Position Statement Cytotherapy 2006, 8: 315–317.Google Scholar
- You R, Li X, Liu Y, Liu G, Lu S, Li M: Response of filopodia and lamellipodia to surface topography on micropatterned silk fibroin films. J Biomed Mater Res A 2014. in press in pressGoogle Scholar
- Mattila PK, Lappalainen P: Filopodia: molecular architecture and cellular functions. Nat Rev Mol Cell Biol 2008, 9: 446–454. 10.1038/nrm2406View ArticleGoogle Scholar
- Small JV, Stradal T, Vignal E, Rottner K: The lamellipodium: where motility begins. Trends Cell Biol 2002, 12: 112–120. 10.1016/S0962-8924(01)02237-1View ArticleGoogle Scholar
- Parker KK, Brock AL, Brangwynne C, Mannix RJ, Wang N, Ostuni E, Geisse NA, Adams JC, Whitesides GM, Ingber DE: Directional control of lamellipodia extension by constraining cell shape and orienting cell tractional forces. FASEB J 2002, 16: 1195–1204. 10.1096/fj.02-0038comView ArticleGoogle Scholar
- Brock A, Chang E, Ho C-C, LeDuc P, Jiang X, Whitesides GM, Ingber DE: Geometric determinants of directional cell motility revealed using microcontact printing. Langmuir 2003, 19: 1611–1617. 10.1021/la026394kView ArticleGoogle Scholar
- Crouch AS, Miller D, Luebke KJ, Hu W: Correlation of anisotropic cell behaviors with topographic aspect ratio. Biomaterials 2009, 30: 1560–1567. 10.1016/j.biomaterials.2008.11.041View ArticleGoogle Scholar
- Bucaro MA, Vasquez Y, Hatton BD, Aizenberg J: Fine-tuning the degree of stem cell polarization and alignment on ordered arrays of high-aspect-ratio nanopillars. ACS Nano 2012, 6: 6222–6230. 10.1021/nn301654eView ArticleGoogle Scholar
- Hotulainen P, Lappalainen P: Stress fibers are generated by two distinct actin assembly mechanisms in motile cells. J Cell Biol 2006, 173: 383–394. 10.1083/jcb.200511093View ArticleGoogle Scholar
- Fletcher DA, Mullins RD: Cell mechanics and the cytoskeleton. Nature 2010, 463: 485–492. 10.1038/nature08908View ArticleGoogle Scholar
- Dalby MJ, Gadegaard N, Tare R, Andar A, Riehle MO, Herzyk P, Wilkinson CDW, Oreffo ROC: The control of human mesenchymal cell differentiation using nanoscale symmetry and disorder. Nat Mater 2007, 6: 997–1003. 10.1038/nmat2013View ArticleGoogle Scholar
- Gronthos S, Brahim J, Li W, Fisher LW, Cherman N, Boyde A, DenBesten P, Robey PG, Shi S: Stem cell properties of human dental pulp stem cells. J Dent Res 2002, 81: 531–535. 10.1177/154405910208100806View ArticleGoogle Scholar
- D'Aquino R, Graziano A, Sampaolesi M, Laino G, Pirozzi G, De Rosa A, Papaccio G: Human postnatal dental pulp cells co-differentiate into osteoblasts and endotheliocytes: a pivotal synergy leading to adult bone tissue formation. Cell Death Differ 2007, 14: 1162–1171. 10.1038/sj.cdd.4402121View ArticleGoogle Scholar
- Punzón-Quijorna E, Sánchez-Vaquero V, Muñoz-Noval Á, Perez-Roldan MJ, Martín-Palma RJ, Rossi F, Climent-Font A, Manso-Silván M, Garcia-Ruiz JP, Torres-Costa V: Nanostructured porous silicon micropatterns as a tool for substrate-conditioned cell research. Nanoscale Res Lett 2012, 7: 396. 10.1186/1556-276X-7-396View ArticleGoogle Scholar
- Kaivosoja E, Myllymaa S, Kouri V-P, Myllymaa K, Lappalainen R, Konttinen YT: Enhancement of silicon using micro-patterned surfaces of thin films. Eur Cell Mater 2010, 19: 147–157.Google Scholar
- Li QS, Lee GYH, Ong CN, Lim CT: AFM indentation study of breast cancer cells. Biochem Biophys Res Commun 2008, 374: 609–613. 10.1016/j.bbrc.2008.07.078View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.